Isostructurality in the Guest Free Forms and in the Clathrates of 1,3,5-Triethyl-2,4,6-tris(4-halophenoxy)methylbenzenes
Bhattacharya, Suman; Saha, Binoy K.; Crystal Growth & Design 12 (2012) 169–; doi:10.1021/cg2009144

data_4502797
_publ_section_title
;
 Isostructurality in the Guest Free Forms and in the Clathrates of
 1,3,5-Triethyl-2,4,6-tris(4-halophenoxy)methylbenzenes
;
_journal_issue                   1
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              169
_journal_paper_doi               10.1021/cg2009144
_journal_volume                  12
_journal_year                    2012
_chemical_formula_moiety         'C33 H33 Br3 O3'
_chemical_formula_sum            'C33 H33 Br3 O3'
_chemical_formula_weight         717.29
_chemical_name_common            1Br
_chemical_name_systematic
;
1,3,5-triethyl-2,4,6-tris(4-bromophenoxy)methylbenzene
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2011-09-21
_audit_creation_method
;
  Olex2 1.1
  (compiled 2011.08.18 svn.r1932, GUI svn.r3819)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 109.733(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   19.1740(6)
_cell_length_b                   13.3687(4)
_cell_length_c                   25.1912(9)
_cell_measurement_reflns_used    7738
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      29.1919
_cell_measurement_theta_min      2.7178
_cell_volume                     6078.1(4)
_computing_cell_refinement
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.66 (release 28-04-2010 CrysAlis171 .NET)
(compiled Apr 28 2010,14:27:37)
;
_computing_data_collection
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.66 (release 28-04-2010 CrysAlis171 .NET)
(compiled Apr 28 2010,14:27:37)
;
_computing_data_reduction
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.66 (release 28-04-2010 CrysAlis171 .NET)
(compiled Apr 28 2010,14:27:37)
;
_computing_molecular_graphics
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_publication_material
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_structure_refinement
;
XL, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_detector_area_resol_mean 15.9821
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.850
_diffrn_measurement_details
;
  1 omega   38.00   82.00   1.0000   12.0000
omega____ theta____ kappa____ phi______ frames
    -       19.2928  179.0000   90.0000 44

  2 omega   25.00   73.00   1.0000   12.0000
omega____ theta____ kappa____ phi______ frames
    -       19.2928 -126.0000  105.0000 48

  3 omega  -34.00   82.00   1.0000   12.0000
omega____ theta____ kappa____ phi______ frames
    -       19.2928    0.0000    0.0000 116

  4 omega    3.00   28.00   1.0000   12.0000
omega____ theta____ kappa____ phi______ frames
    -       19.2928 -107.0000 -174.0000 25
;
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_UB_11      -0.0175683839
_diffrn_orient_matrix_UB_12      -0.0300280473
_diffrn_orient_matrix_UB_13      -0.0240222146
_diffrn_orient_matrix_UB_21      0.0021367877
_diffrn_orient_matrix_UB_22      -0.0418673936
_diffrn_orient_matrix_UB_23      0.0177705628
_diffrn_orient_matrix_UB_31      -0.0351023450
_diffrn_orient_matrix_UB_32      0.0125065640
_diffrn_orient_matrix_UB_33      0.0017674197
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.0672
_diffrn_reflns_av_unetI/netI     0.1905
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_number            28473
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         29.26
_diffrn_reflns_theta_min         2.72
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    4.014
_exptl_absorpt_correction_T_max  0.414
_exptl_absorpt_correction_T_min  0.257
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.33.66 (release 28-04-2010 CrysAlis171 .NET)
(compiled Apr 28 2010,14:27:37)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.568
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2880
_exptl_crystal_size_max          0.36
_exptl_crystal_size_mid          0.29
_exptl_crystal_size_min          0.22
_refine_diff_density_max         1.255
_refine_diff_density_min         -1.131
_refine_diff_density_rms         0.121
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.823
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     709
_refine_ls_number_reflns         16564
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.823
_refine_ls_R_factor_all          0.1381
_refine_ls_R_factor_gt           0.0485
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0328P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0788
_refine_ls_wR_factor_ref         0.0902
_reflns_number_gt                6466
_reflns_number_total             16564
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg2009144_si_001.cif
_cod_data_source_block           1Br
_cod_original_cell_volume        6078.1(3)
_cod_database_code               4502797